Synthesis of Photoactive Materials by Sonication: Application in Photocatalysis and Solar Cells
- 2.5k Downloads
In recent years, a good number of methods have become available for the preparation of an important group of photoactive materials for applications in photocatalysis and solar cells. Nevertheless, the benefits derived from preparing those materials through unconventional approaches are very attractive from the green chemistry point of view. This critical review work is focused on sonication as one of these promising new synthetic procedures that allow control over size, morphology, nanostructure and tuning of catalytic properties. Ultrasound-based procedures offer a facile, versatile synthetic tool for the preparation of light-activated materials often inaccessible through conventional methods.
KeywordsPhotoactive materials by sonication Photocatalysis Ultrasounds Solar cells Perovskites Quantum dots
Reactive black 5
Volatile organic compounds
Ultrasonic spray pyrolysis
Electron spin resonance spectroscopy
Quantum dot sensitized solar cells
Perovskite solar cells
Power conversion efficiency
Dye sensitized solar cells
Reactive oxygen species
Ultrasound treatment technique
Substrate vibration-assisted drop casting method
Indium tin oxide
N 2,N 2,N 2 ′ ,N 2 ′ ,N 7,N 7,N 7 ′ ,N 7 ′ -octakis(4-methoxyphenyl)-9,9′-spirobi[9H-fluorene]-2,2′,7,7′-tetramine
1 Sonochemical Preparation of Photoactive Catalytic Materials
The phenomenology of fabrication of highly efficient photocatalysts through an ultrasound route represents a very interesting and important area in science and technology, and it holds great potential for photocatalysts preparation in the near future [1, 2, 3]. In comparison with traditional sources of energy, ultrasound ensures unusual reaction conditions in liquid phase reactions due to the cavitation phenomenon (extremely high temperatures and pressures are formed in very short times in liquids) [3, 4]. Furthermore, application of ultrasound irradiation to a photocatalytic system might enhance both the bulk and localized mass transport and consequently expedite the molecular contact and the photocatalytic activity [1, 2, 4, 5, 6]. A considerable number of novel photocatalysts with novel nano-/microstructures (e.g., ZnWO4 , CdMoO4 , V2O5 , CuMoO4 , TiO2/Bi2O3 ) have been prepared by means of ultrasound-assisted methodology. In this subsection, we would like to focus the readers’ attention on ultrasound-promoted procedures for the preparation of photocatalysts, and the potential application of these materials in the photocatalytic degradation and selective oxidation of organic compounds.
1.1 Sonochemical Synthesis of TiO2 Photocatalyst
Selected research studies of ultrasound assisted processes in the synthesis of photocatalysts and photoactive catalytic materials
15 W mL−1
0.5, 1, 2, 4 and 8 h at 80 °C, 100 mL
Totally disorder structure of amorphous TiO2 both before and after ultrasonic treatment was observed
45 kHz, 60 W
Ambient conditions for 10 h, glass tube sealed with a screw cap
CaTiO3 and BaTiO3 nanoparticles with almost regular spherical shape and uniform particle size (~20 nm) were observed. SrTiO3 particles were found to agglomerate more strongly leading to cubic-like aggregates with edge lengths varying (100–300 nm)
12 mm diameter Ti horn, 75 W, 20 kHz
1, 1.5, 2, 3, and
4 h at RT, 150 mL
The nanocomposites prepared by 2 h ultrasonic irradiation have the best activity
12 mm diameter Ti horn, 75 W, 20 kHz
0.5, 1, 2, and 4 h
at RT, 150 mL
Photocatalyst prepared by ultrasonic irradiation for 1 hour has superior activity compared to other samples, and has remarkable stability and excellent magnetic filtration from the treated solutions
12 mm diameter Ti horn, 75 W, 20 kHz
0.25, 0.5, 1, 2, and 3 h at RT, 150 mL
Material prepared by ultrasonic irradiation for 1 h has the superior activity
12 mm, 33 Hz,
5 h at ambient
temperature, 150 mL
g-C3N4 sheet possesses porous structure with high surface area and large pore volume
Worth mentioning is the work by Mao et al.  on the preparation of mesoporous titanium dioxide (TiO2) inside the periodic macropores of diatom frustules by sonochemical condensation of titania precursor, and then thermal treated at elevated temperatures, resulting in hierarchical macro/mesoporous materials. Furthermore, hierarchical structure provides a large number of accessible active sites for efficient transportation of guest species to framework binding sites. It was found that a high photocatalytic degradation of methylene blue as compared with P25 can be achieved with the composite having a certain loading amount of TiO2 (30 wt%), attributing to its hierarchical macro/mesoporous structures. It should be also noted that mesoporous titanium TiO2 with wormhole channel together with interconnected 3D structures inside diatom pores prepared by sonochemical synthesis with organic surfactant as structure directing agent has potentially important structural features for photocatalytic reactivity, because channel branching within the framework may facilitate access to reactive sites on the framework wall, which is most critical for its use as photocatalyst.
In terms of improvement of TiO2 photocatalytic properties under solar light by means of a suitable modification, enhanced photocatalytic activity of TiO2 nanocomposites for the degradation of dyes and Gram negative bacteria (Escherichia coli) was obtained by doped TiO2 with Al2O3, Bi2O3, CuO and ZrO2  and synthesized via sonochemical method. It is interesting to notice that Bi2O3–TiO2 nanocomposite is more efficient toward the degradation of the dyes under solar light and TiO2 is the least efficient photocatalyst; the efficiency is in the order: Bi2O3–TiO2 > Al2O3–TiO2 > CuO–TiO2 > ZrO2–TiO2 > TiO2. It should be also noted that the antibacterial activity of all the five synthesized nanocomposites was tested against Gram negative bacteria (E. coli) by varying the concentrations (250, 500, 750 and 1000 µg). Among them, Al2O3–TiO2 shows some significant zone of inhibition around the film under dark condition. Recently, certain novel promising photocatalysts prepared by ultrasound-assisted method have been described in several research papers and review articles [1, 2, 3].
1.2 Sonochemical Synthesis of Selected Photocatalysts
Sonochemical method has been used extensively to generate novel materials with unusual (photo)-catalytic properties, due to its unique reaction effects. For example, addition of titanium iso-propoxide induces the generation of new linear polymeric chains type nickel-titanium-ethylene glycol (Ni–Ti–EG), as revealed by the color change (from green to light blue). This light blue polymer coagulates to form a uniform rod-like precursor by van der Waals interactions . Another elegant strategy to prepare ternary CaTiO3, SrTiO3 and BaTiO3 materials by a one-step room-temperature ultrasound synthesis in ionic liquid for photocatalytic applications (photocatalytic hydrogen evolution and methylene blue degradation) was recently described  (Table 1, Entry 2). It is also important to note that the use of ionic liquids in sonochemistry is advantageous due to their low measurable vapor pressure, low viscosity, low thermal conductivity, and high chemical stability, which are all significant parameters to generate efficient cavitation.
Photoactive materials such as SrZrO3have been recently explored because they exhibit suitable properties for photocatalytic hydrogen evolution from water splitting . The results confirm that SrZrO3 was stable with time of hydrogen evolution and a very high rate (35 µmol g−1 h−1) was exhibited by SrZrO3 prepared by ultrasound-assisted synthesis. Recently, multiferroics such as BiFeO3 (BFO) are worthy of notice due to their unique and strong coupling of electric, magnetic, and structural order parameters in terms of practical applications, since both ferroelectric and antiferromagnetic ordering temperatures are well above room temperature (Curie temperature 830 °C and Neel temperature 370 °C) . Moreover, other researchers have applied BFO materials prepared by sono-synthesis with high photocatalytic activity under solar light in degradation of various compounds such as Rhodamine B , methylene blue , Reactive Black 5 (RB5)  and phenolic compounds . As anticipated above, BiFeO3 nanoparticles with measured band gap of 2.0 eV synthesized with ultrasound exhibited higher crystallization, smaller crystallite size and higher photocatalytic activity than the material synthesized with conventional methods.
Previous research  showed that orthorhombic stannous sulfide (SnS) nanoparticles synthesized via a sonochemical route by 20 kHz sonication had smaller crystalline size (4 ± 1 nm) in comparison to the nanoparticles that were synthesized by 50 kHz sonication (6 ± 1 nm). An optical investigation confirmed that the SnS particles had strong emission bands located at the UV and visible regions, suggesting that they have the potential to be used as optical devices.
It is known that n–n heterojunctions between two n-type semiconductors can effectively promote separation of photogenerated electron–hole pairs, due to formation of internal electric field. Hence, preparation of ZnO/Ag3VO4 nanocomposites prepared by an ultrasonic-assisted one-pot method led to the enhanced photocatalytic activity for organic pollutants degradation under visible-light irradiation  (Table 1, Entry 3). Interestingly, photocatalytic activity of ZnO/Ag3VO4 nanocomposite under visible-light irradiation is about 21, 56, and 2.8-fold higher than that of the ZnO sample in degradation of rhodamine B, methylene blue, and methyl orange, respectively. Furthermore, it was revealed that the photocatalytic activity was attributed to greater generation of electron–hole pairs due to photosensitizing role of Ag3VO4 under visible-light irradiation and the efficient separation of the photogenerated electron–hole pairs due to formation of n–n heterojunction between the counterparts. Previous studies  (Table 1, Entry 4) showed that photocatalytic activity of the ZnO/AgI/Fe3O4 nanocomposite in degradation of rhodamine B, methylene blue, and methyl orange is about 32-fold higher than that of the ZnO/Fe3O4 sample prepared by ultrasonic irradiation method. The highly enhanced activity of novel ternary ZnO/AgI/Fe3O4 magnetic photocatalyst was mainly attributed to visible-light harvesting efficiency and decreasing recombination of the charge carriers as well. It should be noted that ultrasonic irradiation time and calcination temperature largely affect the photocatalytic activity. In another investigation  (Table 1, Entry 5), it was found that ternary ZnO/AgI/Ag2CrO4 photocatalyst with 20 % of Ag2CrO4 is active in rhodamine B degradation, with nearly 167-, 6.5-, and 45-fold higher conversion than that of ZnO, ZnO/AgI, and ZnO/Ag2CrO4, respectively, materials also prepared by ultrasonic irradiation method. Furthermore, visible-light activity of ZnO/AgI/Ag2CrO4 is about 6.5-, 16-, and 33-fold higher than that of the ZnO/AgI, whereas 45-, 22-, and 136-fold higher than that of the ZnO/Ag2CrO4 in degradation of rhodamine B, methylene blue, and methyl orange, respectively. It should be pointed out that photocatalyst prepared by ultrasonic irradiation for 60 min has the superior activity.
Recently, metal-free graphitic carbon nitride (g-C3N4) was synthesized via facile template-free sonochemical route and enhanced photodegradation of rhodamine B  (Table 1, Entry 6). The authors found that mesoporous g-C3N4 (112.4 m2 g−1) has almost 5.5 times higher photoactivity than that of bulk g-C3N4 (8.4 m2 g−1) under visible-light irradiation, which is attributed to the much higher specific surface area, efficient adsorption ability and the unique interfacial mesoporous structure that can favor the absorption of light and separation of photoinduced electron–hole pairs more effectively. Additionally, reactive oxidative species detection studies indicated that the photodegradation of rhodamine B over mesoporous g-C3N4 under visible-light is mainly via superoxide radicals.
Zhou et al.  prepared Zn3V2O7(OH)2(H2O)2 and g-C3N4/Zn3V2O7(OH)2(H2O)2 using sonochemical method with high photocatalytic activities in degradation of methylene blue. Interestingly, the absorption edge of g-C3N4/Zn3V2O7(OH)2(H2O)2 had red shift reaching 450 nm, and a significantly enhanced photocatalytic performance in degrading methylene blue, which increased to about 5.6 times that of pure Zn3V2O7(OH)2(H2O)2. During the ultrasound process, the heterojunction structure of g-C3N4/Zn3V2O7(OH)2(H2O)2 was formed and this special structure increased the separation efficiency of photogenerated electron–hole pairs, resulting in the enhancement of photocatalytic performances. Table 1 shows some detailed information about ultrasound assisted synthesis methods of photocatalysts made by selected research groups.
Another approach offering prospects for preparation of nanostructured TiO2/STARBON®-polysaccharide-derived mesoporous materials by means of ultrasound-assisted wet impregnation method was investigated . Interestingly, carboxylic acid groups can be formed on the surface after initial thermal treatment at 400 °C under an oxygen-deficient atmosphere. Each carboxyl acid group acts as an individual nucleation site for TiO2 formation, which is possible under hydrolysis and condensation reactions promoted by sonication. Finally, the hybrid material (TiO2/STARBON®) is consolidated after thermal treatment at 400 °C. These conditions preserve pure, highly crystalline anatase phase (ca. 30 nm), leading to a reduction in the electron–hole recombination rate at the Starbon surface. TiO2 nanoparticles are strongly anchored and have good contact with the STARBON-800 structure (i.e., no leaching after 240 min of photocatalytic degradation of phenol), believed to enhance the photoelectron conversion (i.e., as compared with Norit and Graphene oxide supports) of TiO2 by reducing the recombination of photo-generated electron–hole pairs.
A similar study using a simple and effective ultrasound-assisted wet impregnation method was developed for the preparation of magnetically separable TiO2/maghemite-silica photo-active nanocomposites tested in the liquid phase selective oxidation of benzyl alcohol . Interestingly, photocatalytic selectivity in organic media (90 % in acetonitrile) towards benzaldehyde was achieved at a benzyl alcohol conversion of ca. 50 %. Solvents played a significant role in the photo-oxidation process with materials showing very good conversion and selectivity in acetonitrile but not in aqueous conditions. Additionally, spatially ordered heterojunction between TiO2 and γ-Fe2O3 and a potential co-catalytic incorporation of Fe3+ into the TiO2 structure might significantly increase the sensitization and decrease the band gap energy of TiO2, effectively improving the photocatalytic activity and selectivity of these photocatalysts.
In an attempt to better understand the sonophotodeposition method (SPD), the iron-containing TiO2/zeolite-Y photocatalyst for the selective oxidation of benzyl alcohol was investigated . Generally, photocatalyst prepared by the sonophotodeposition method showed better results, in terms of alcohol conversion and yield of benzaldehyde, in comparison with the photocatalyst prepared by an ultrasound-assisted wet impregnation method. Furthermore, sonication probe and sun-imitating Xenon lamp were tested, and for the first time, a non-noble metal was deposited on the TiO2 surface by using visible light, but with the help of ultrasound. It is worth noting that sonophotodeposition method is an innovative, simultaneous combination of ultrasonication and ultraviolet irradiation, and is highly energy efficient. Reactions can be carried out at room temperature and atmospheric pressure, very short reaction times and without using strong chemical reduction agents. Additionally, a considerable number of novel mono and bimetallic photocatalysts (e.g., Pd/TiO2 , Pd-Au/TiO2 , Pd-Cu/TiO2 ) have been prepared by sonophotodeposition methodology for selective oxidation of volatile organic compounds (VOCs).
1.3 Ultrasonic Spray Pyrolysis for the Preparation of Photocatalysts
Ultrasonic spray pyrolysis (USP) method is a low-cost, continuous operation, and environmentally benign process with short processing time, which has been used to synthesize functional materials . A distinctive feature of the method is that it can produce porous microspheres of various compositions without template and with good phase purity, and the morphology can be easily controlled during the process to ensure homogeneous composition distribution in the spheres [52, 53]. In this approach of ultrasonic spray pyrolysis, Suslick et al.  synthesized BiVO4 powders with particles ranging from thin, hollow and porous shells to ball-in-ball–type structures. Interestingly, materials prepared by USP are more active for oxygen evolving photocatalysts under visible-light irradiation (λ > 400 nm) in AgNO3 solution than commercial BiVO4 and WO3 powders, likely due to differences in the particle morphology. It was found that the increase of photocatalytic activity is likely due to the short distances electron–hole pairs must move to reach the surface in order to perform the desired redox reactions. Recently, USP was adapted to fabricate hierarchical porous ZnWO4 microspheres and evaluated by the degradation of gaseous NO x under simulated solar light irradiation . It was found that synthesis temperature (650–750 °C) was a key factor influencing the microstructures of resulting ZnWO4 samples, eventually affecting their photocatalytic activity, and which could be explained by improved optical absorption capability, high specific surface area, and fast separation/diffusion rate of the photogenerated charge carriers. Additionally, electron spin resonance spectroscopy (ESR) method indicated that O 2 ·− and ·OH radicals function as the major reactive species for NO x decomposition. Compared to solid spheres, hollow PbWO4 spheres, which combine the merits of hollow and porous structures, could present improved mass transfer and high surface areas . Moreover, hollow structured PbWO4 spheres exhibited superior photocatalytic activity to solid spheres (NO removal rate is 35 ppb min−1), due to the differences in microstructure and morphology.
2 Perovskite Solar Cells and Quantum Dots Photovoltaics
The interest in sonochemistry as a versatile tool for materials synthesis has been increasing, especially in the case of preparation of nanostructured materials for energy conversion like quantum dots, solar photovoltaic cells and dye-sensitized solar cells [59, 60]. The application of ultrasound allows to obtain a uniform shape and highly pure nanoparticles with a narrow size distribution, which has influence on the unique characteristics of photovoltaic devices. Additionally, ultrasound-assisted methodologies can decrease the time of synthesis, consequently reducing operating costs and develop effective manufacturing processes [60, 61]. Hence, it is a promising inexpensive alternative for the production of the next generation of solar cells such as quantum dot sensitized solar cells (QDSCs) or perovskite solar cells (PSCs) . Perovskites are a class of compounds that possess well-defined crystal structure with formula ABX3, where, the A and B sites are engaged by cations and the X site is occupied by the anion. Depending on the type of the ions, they can form various perovskite crystal geometries with different features. The cations in the lattice are able to enhance and modify the band structure, which is particularly important from the point of view of photophysical properties [63, 64]. Thus, perovskites as an active layer in photovoltaic systems can deliver high open-circuit voltages and lead to the harvesting of light from a broad spectrum . Perovskite solar cells are able to absorb the shorter wavelengths of visible light corresponding to photons with higher energy. Consequently, they can reach the maximum voltage of cells adequate to the maximum electrical power that comes from incident photons. Therefore, PSCs that stem from dye-sensitized solar cells (DSSCs) are considered as a forerunners of emerging photovoltaic technology [64, 65].
Perovskites first used for solar applications were documented in a seminal article by Miyasaka and co-workers in 2009 , and then by Park and co-workers 2 years later . In all cases, the perovskite solar cells emerge as long-running, durable photovoltaic devices with high efficiency, and have been increasing from 10 to 20 % in the last few years [68, 69]. Due to fact that PCSs possess an enhanced light-harvesting system, improved charge separation process as well revised charge transfer and charge collection [68, 69], the power conversion efficiency (PCE) of perovskites solar cells is remarkable higher compared to the previous generation solar cells devices [i.e., wafer-based silicon devices or thin film SCs made from cadmium telluride (CdTe)]. The properties mentioned above can be attributed to the special structure of these materials, which mainly reflect on their application of photovoltaic technology as well as of other domains .
The next interesting possibility leading to more efficiently working solar cells is the development of quantum dot sensitized solar cells. It is worth noting that the energy conversion of solar cells directly depends on their structure, i.e., conductive substrates, semiconducting layers and in particular, sensitizing molecules (dye or quantum dots). The structure of DSSCs is similar to that of QDSCs; however, the power conversion efficiency (PCE) is remarkably lower in the case of QDSCs. Nevertheless, due to the relatively low cost related to using inexpensive semiconductors and a simple fabrication, possible approaches for improving PCE are still under debate [61, 62, 71].
In this subsection, we would like to focus the readers’ attention on the use of sonochemical methodology as a convenient tool for the preparation of solar cells with higher power conversion efficiency; indicating the influence of ultrasounds on the formation of quantum dots and perovskite solar cells, and pointing out the current state of the art.
2.1 Sonochemical Synthesis of Perovskites and Quantum Dots
The wide range of sonochemical methods used for the synthesis of perovskite-type oxides ABO3 have been well reviewed by Colmenares group . Among the most effective sonication-based processes, we can distinguish mainly co-precipitation methods, sol–gel methods, and hydrothermal methods as well aerosol synthetic techniques [e.g., the ultrasonic spray pyrolysis (USP)]. In comparison with conventional methodologies, which are mentioned above, the USP allows for control over size and shape of particles in a simple and more reproducible way. The selection of optimal parameters (such as ultrasound frequency, characteristic of the precursor solution and temperature) allows a nanomaterial with desirable properties to be obtained. However, it is not the only effective approach for the preparation of thin-films and ultrafine nanostructures in terms of manufacturing photovoltaic devices. An interesting concept that involves combination of ultrasonic spray technique and thermal evaporation process was reported by Xia et al. . The modified deposition method assisted by ultrasonic spray coating used for the formation of CH3NH3PbI3 thin film layers enables control of morphology. The obtained perovskite film possesses larger crystal size (>500 nm), which result in higher carriers mobility and lower charge recombination. Thereby, uniform coverage prevents an undesirable short circuit between the top and back surface contacts of a solar cell, resulting in an increase in the power conversion of photovoltaic devices .
Selected examples of sonochemical methods applied for the synthesis of active solar cells layers
The ultrasonic transducer (frequency 20 kHz) was operated at an amplitude of 60 %
Time of irradiation increased from 10 to 30 min
The CH3NH3PbI3 nanoparticles of polygonal shapes in the size range of 10–40 nm were obtained until 20 min reaction, whereas the shorter time of irradiation resulted in non-uniform shapes
A multiwave ultrasonic generator equipped with titanium oscillator (12.5 mm) operating at 20 kHz
Power of ultrasound was adjusted in the range from 50 to 70 W
The particle size of CuInS2 was about 100 nm when the power of ultrasound was equal to 50 W—increasing the power led to formation of uniform particles with size of 60 nm
A sonication system operated at 59 kHz and a power output of 99 W
Concentration of precursor and sonication time (various variants)
The desired kesterite phase of CuZnSnS2 was obtain using longer time of irradiation and higher precursor concentration
A ultrasound probe (frequency 20 kHz, 130 W/cm2) operated at 50 % amplitude
The effect of ultrasound on the reduction process
The reduction process of tellurium does not exceed 15 min and allows to obtain CdTe QDs with the band gap value (2.3 eV)
Ultrasound horn with 1.9 cm diameter (20 kHz, output acoustic power 45.5 W)
The sonication time (0–45 min) and temperature (40–60 °C)
The CdS nanoparticles have uniform spherical morphology with size around 2 nm (60 °C after 45 min of irradiation).
The one-step sonochemical method proposed by Liu et al.  can be applied for the production of Cu2ZnSnS4 perovskites (Table 2; Entry 3). By this way, the propitious shape of nanoparticles can be obtained by facile and rapid synthesis through the selection of an optimal precursor’s concentration as well the above-mentioned sonication time . However, in the event of the production of high quality inks for solar-cells fabrication, a more suitable methodology seems to be the ultrasound-assisted microwave solvothermal method. Unlike the others, the nucleation–dissolution–recrystallization mechanism allows to obtain Cu2ZnSn4 nanosized particles with hexagonal prisms structure, due to fact that the synergistic effect of ultrasound and microwave plays a key role in the growth process of wurtzite phase [83, 84].
Ultrasound-assisted processes are also used to prepare quantum dot particles (QDs) for solar cells application. The simple and fast sonochemical methodology provides monodispersed CdTe QDs with a strong quantum confinement regime (Table 2; Entry 4). The application of ultrasound allows one to control the morphology and reduce the surface defects of quantum dots. As a result, this allowed the production of nanoparticles with only one fluorescence band, which is beneficial in terms of photovoltaic devices . Furthermore, it is clearly shown that the application of ultrasound, in particular the sonication time, has an influence on the particle size distribution and the growth kinetics (Table 2; Entry 5) . Results indicate that the increase of particle size at longer time is attributed to the diffusion-limited coarsening process, which is accelerated by cavitation. Thus, the effect of ultrasound irradiation causes that the synthesis of QDs nanoparticles occurs in shorter time using low temperature methodology such as the micro-emulsion method . Additionally, sonochemically synthesized QDs possess better optical properties and are able to produce a large amount of reactive oxygen species (ROS), which may influence a further course of the photochemical processes .
2.2 Sonochemical Solar Cells Fabrication
Sonochemical methodology can be used as the first step toward the synthesis of photoactive layers or as the second step for the preparation of solar cells devices. The wide range of ultrasound parameters (i.e., ultrasonic power, frequency and time) have a positive influence on the size, morphology, structure or the surface area, and in consequence on optical as well as electrical properties of photovoltaic devices . It was proven that the ultrasound irradiation accelerates the nucleation process, and promotes ionic and mass diffusion, which permit the synthesis of structures with desirable features in terms of the photovoltaic application . For this reason, ultrasounds play a crucial role in the preparation of solar cells structures and cells’ components.
The photoactive layers can consist of perovskite nanoparticles, quantum dots or hierarchical hollow spheres which can improve the efficiency of dye-sensitized solar cells (DSSCs), or quantum dots solar cells . The DSSCs type of solar cells exhibited significant better parameters (i.e., a short circuit current density, open circuit voltage and fill factor) in comparison to standard nanoparticle photoelectrode, consequently increasing the power conversion efficiency and photocatalytic performance . The hierarchical structures (HSs) (mainly ZnO, TiO2, SnO2) synthesized through the sonochemistry methodology demonstrate required properties caused by their nano/micro combined architectures. They enable fast electron transport due to an ideal network created by nanosheets connection. Additionally, HSs possess a large surface area, which improves the accessibility for incident photons [88, 91]. Furthermore, dye-sensitized solar cells based on hierarchical structures are able to enhance the light harvesting capability and improve the efficiency of SCs . Using ultrasound treatment technique (UST), the change of the solar power efficiency can be improved up to 50 % .
Prof. Dr. Juan C. Colmenares would like to thank the National Science Centre (Poland) for support within the project Sonata Bis Nr. 2015/18/E/ST5/00306. Paweł Lisowski would like also to thank the National Science Centre (NCN) in Poland for the research project 2015/17/N/ST5/03330.
- 60.Babu SG, Neppolian B, Ashokkumar M (2015) Ultrasound assisted synthesis of nanoparticles for energy and environmental applications. In: Ashokkumar M (ed) Handbook of ultrasonics and sonochemistry, 1st edn. Springer, Singapore, pp 1–34Google Scholar
- 61.Kim H (2012) Ultrasonic synthesis of materials for energy conversion devices. Dissertation, University of California University of IllinoisGoogle Scholar
- 69.Jasim KE (2015) Quantum dots solar cells. In: Kosyachenko LA (ed) Solar cells—new approaches and reviews, 1st edn. InTech, pp 304–329. doi: 10.5772/59159
- 72.Colmenares JC, Magdziarz A, Lisowski P (2015) Application of microwave and ultrasound irradiation in the synthesis of perovskite-type oxides ABO3. In: Granger P, Parvulescu VI, Parvulescu VI, Prellier W (eds) Perovskites and related mixed oxides concepts and applications, 1st edn. Wiley, Weinheim, pp 91–113Google Scholar
- 73.Xia Z, Chai G, Wang Y, Zhou H (2015) Uniform perovskite photovoltaic thin films via ultrasonic spray assisted deposition method. In: Photovoltaic Specialist Conference (PVSC), New Orleans, IEEE, pp 1–4Google Scholar
- 77.Lishan SJ, Tong D, Qingbiao L, Yong T (2007) Study of photocatalytic performance of SrFeO3x by ultrasonic radiation. Catal 8:963–966Google Scholar
- 79.Wattanawikkam CH, Pecharapa W (2015) Optical, dielectric and photocatalytic properties of perovskite ZnTiO3 nanoparticle synthesized by sonochemical process. In: Joint IEEE International Symposium on the Applications of Ferroelectric, International Symposium on Integrated Functionalities, and Piezoelectric Force Microscopy Workshop, Singapore, IEEE, pp 280–284Google Scholar
- 86.Ghows N, Entezari MH (2013) Quantum sots of CdS synthesized by micro-emulsion under ultrasound: size distribution and growth kinetics. Phys Chem Res 1:166–174Google Scholar
- 94.Tait JG, Manghooli S, Qiu W, Rakocevic L, Kootstra L, Jaysankar M, Masse de la Huerta CA, Paetzold UW, Gehlhaar R, Cheyns D, Heremans P, Poortmans J (2016) Rapid composition screening for perovskite photovoltaics via concurrently pumped ultrasonic spray coating. J Mater Chem A 4:3792–3828CrossRefGoogle Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.